Download presentation

Presentation is loading. Please wait.

Published byPorter Napier Modified over 2 years ago

1
1 Results of Conductor Testing in SULTAN: A Review R. Wesche, M. Bagnasco, P. Bruzzone, M. Calvi, F. Cau, R. Herzog, C. Marinucci, B. Stepanov EPFL – CRPP, Switzerland Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008

2
2 Introduction Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 In the last few years a large number of NbTi and Nb 3 Sn sub- as well as full-size cable-in-conduit (CIC) conductors were tested in the SULTAN facility. For many of these conductors, the strand critical current was measured separately as a function of field, temperature and strain. Using strand scaling relations (interpolation) and the measured strand data the potential DC performance of various CIC conductors has been estimated. In the estimation of the potential T cs or I c it has been supposed that the current distribution is uniform. The performance of the SULTAN samples is compared to this potential performance.

3
3 SULTAN Samples Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Sub-size (hairpin) samples (No bottom joint) Full-size samples (With bottom joint) He L: T11/T11a R: T12/T12a L: T9/T9a R: T10/T10a L: T7/T7a R: T8/T8a L: T5/T5a R: T6/T6a L: T3/T3a R: T4/T4a

4
4 Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 NbTi CIC Conductors CICCStrandCoatingCable patternN NbTi NbTi #1ANi (1NbTi+7Cu) NbTi #2BSnAg (1Cu+6NbTi) NbTi #3BNi (1Cu+6NbTi) NbTi #4BNi & wraps (1Cu+6NbTi) NbTi #5CNi (1Cu+6NbTi) PFIS LDNi & wraps ( ) 6 NbTi 1440 PFIS RDNi ( ) 6 NbTi 1440 LCJDNi (1Cu+9NbTi) NbTi #3 PFIS R LCJ

5
5 Results of NbTi Sub-size Conductors Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Measured T cs values of NbTi hairpin conductors are very close to the potential T cs. Deviations are of the order of 0.1 K. Cyclic loading does not affect the T cs. 4 out of 5 conductors reach more than 90% of the potential I c. NbTi #4 (wraps): 80% of potential I c. n cable n strand I 9 kA 3% 10% 5% 7% 6% 4%

6
6 Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Results of NbTi Full-size Conductors Measured T cs values of NbTi full-size conductors are in very good agreement with the potential T cs. Deviations are typically less than 0.1 K. All NbTi full-size conductors reach more than 90% of the potential I c. 13% 11%

7
7 Summary NbTi CIC Conductors Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 No significant cyclic load degradation. In 4 out of 8 conductors more than 95% of the potential I c is reached. In 7 out of 8 conductors more than 90% of the potential I c is reached. In NbTi #4 (wraps) only 80% of the potential I c is reached. The deviations from the potential I c include: Accuracy of the strand measurements (Strand B, 0.02 K, 5% in I 6 K, 6 T). Errors in strand scaling parameters ( I c typically below 8%, 6 T underestimation, 6 T overestimation of I c ). Accuracy of the SULTAN temperature measurements before 2006 ( 0.05 K, NbTi #3, 10% in I 6 K, 6 T). Uncertainty in the potential I c, which is based on a completely uniform current distribution and the assumption that each strand is found with the same probability at any position in the cable cross-section.

8
8 Nb 3 Sn Sub-size CIC Conductors Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 CICCStrandDimensions (mm)Twist Pitch (mm) Cable patternN sc VAC Sub- size VAC CSMC 14.5 / / /76/136/ (braid) × Dipole Pre- Prototype OST , × 7.7 Jacket 16.4 × 5.7 Cable 58/95/139/ Cu 84 PITSAM 1OST dipole 21.1 × 9.5 Jacket 17.9 × 6.3 Cable 58/95/139/ PITSAM 2OST dipole 12.6 × 12.6 Jacket 9.1 × 9.1 Cable 58/95/139/ Cu 48 PITSAM 3OST dipole 15.4 × 10.5 Jacket 11.9 × 7 Cable 58/95/139/ Cu 48 PITSAM 5OST dipole × Jacket 9.1 × 9.1 Cable 34/95/139/213 83/140/192/213 3×3×3×4 60 Cu 48

9
9 Dipole Pre-Prototype Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Measured T cs values are close to the potential T cs for = -0.61%. Cable n values above 20 for I c values higher than 20 kA. All measured I c values are close to the potential I c for = -0.61% (no BI dependent extra strain required). Negligible cyclic load degradation.

10
10 PITSAM 1 Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Measured T cs values are close to the potential T cs for = -0.65%. Again the cable I c is close to the potential I c for a single value. In the further considerations a strain of -0.65% is used to calculate the potential T cs or I c values.

11
11 VAC Nb 3 Sn: Triplet versus Braid Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Braid results are closer to the potential T cs and I c values. Moreover, the triplet CICC shows reduced performance after cyclic loading. n values 10.5 T, 11.5 B Braid:I 15 kA I c cable : 80-90% I c pot Triplet:I 15 kA I c cable : 75% I c pot (after cyclic loading) : to -0.90% would fit the data

12
12 Effect of Load and Thermal Cycles Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Considerable performance loss of PITSAM 2 (square conductor) during cyclic loading. CICC half length with long twist pitches shows better performance and less sensitivity to load and thermal cycles. Behavior of PITSAM 3 (aspect ratio: 1.7) is comparable to that of PITSAM 5 long.

13
13 Summary: Nb 3 Sn Sub-size CIC Conductors Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Pre-Prototype and PITSAM 1 reach the potential performance. VAC braid, PITSAM 3 and PITSAM 5L reach 80% of the potential performance. VAC Triplet, PITSAM 2: 70% PITSAM 5S: 55% Pre-Prototype and PITSAM 1 are characterized by good performance and negligible cyclic load degradation. The complete data set can be described by a single value of strain. A rectangular shape seems to be advantageous. Low performance is accompanied by sensitivity to cyclic and thermal loads.

14
14 Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 CICCStrandDimensions (mm)Twist Pitch (mm)Cable patternN sc TFAS 1 L: EAS R: OST2 40.4, /87/126/166/4153×3×5×4×6 (2sc+1Cu)×3×5× TFAS 2L: OCSI R: OKSC 40.4, /87/126/166/4153×3×5×4×6 (2sc+1Cu)×3×5× TFPRO 1L: EAS R: EAS 43.45×43.45, ×42.05, /87/126/245/460(2sc+1Cu)×3×5×5+C)×6 C: 3×4Cu 900 TFPRO 2L: OST2 R: OST ×41.45, ×42.05, /182/245/415/440 45/87/126/245/460 (2sc+1Cu)×3×5×5+C)×6 C: 3×4Cu 900 JATF 1L: Mitsubishi R: Hitachi 43.9×43.9, ×85×130×250×450(2sc+1Cu)×3×5×5+C)×6 C: 3×4Cu 900 JATF 2L: Hitachi R: Mitsubishi 42.7×42.7, ×85×130×250×450(2sc+1Cu)×3×5×5+C)×6 C: 3×4Cu 900 JATF 3L: JASTEC R: Furukawa 42.65×42.65, ×142×178×300×420(2sc+1Cu)×3×5×5+C)×6 C: 3×4Cu 900 KOTFL: KAT R: KAT 43.7×43.7, ×43.7, ×80×125×240×450(2sc+1Cu)×3×5×5+C)×6 C: 3×4Cu 900 RFTF NEFFS Bochvar 43.7×43.7, ×84×124×250×453 Void f: L33%, R32% (2sc+1Cu)×3×5×5+C)×6 C: 3×4Cu 900 TFUS 1 Alternate L: Luvata R: Luvata 43.8×43.8, ×43.8, ×86×127×254×457 25×127×254×457 ITER pattern {[(6sc+1Cu)×6+C1]×5+C2}× Nb 3 Sn Full-size CIC Conductors

15
15 TFAS Nb 3 Sn Full-Size Conductors Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 TFAS OST shows the most pronounced reduction of T cs after cyclic loading. Smaller effects for TFAS EAS and OKSC. Nearly unchanged values for TFAS OCSI. I c values after cyclic loading reach 80% of the potential I c. TFAS OKSC after cyclic loading I c 0.7 I c potential

16
16 TFPRO 1 & 2 Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Both legs of TFPRO1 are close to the potential T cs. The data suggest that the strain is close to -0.6%. Cyclic load effects are negligible. The T cs values measured for TFPRO2 OST2 are far above the potential T cs. No evidence for cyclic load degradation. TFPRO2 OST1 showed a pronounced cyclic load degradation. The lowest T cs value in the plot corresponds to 65% of the potential I c.

17
17 JATF 1, 2 & 3 Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 JATF1: Negligible cyclic load effects. Measured T cs values slightly below the potential T cs. Both the Hitachi and the Mitsubishi leg reach more than 80% of the potential I c. JATF 2 results are in line with the test of JATF 1. Hitachi: 85% of I c pot Mitsubishi: 90% of I c pot JATF 3: T cs of both legs is well below the potential T cs. Evidence for cyclic load degradation. I c of both legs 70% of I c pot (after cyclic loading)

18
18 Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Summary: Nb 3 Sn Full-size CIC Conductors TFAS1-EAS, OST & OKSC: Ratio depends on current. Extra strain or degradation and lower strain. TFPRO1: Both legs are close to the I c pot. Strain is lower than -0.65%. TFPRO2-OST2: Data are consistent with -0.45%. Both legs of TFPRO1 and TFPRO2-OST2 reach I c pot. JATF 1 & 2 Hitachi as well as Mitsubishi are close to I c pot. All 4 TFAS legs, TFPRO2-OST1, JATF3-F & J, and KOTF-L & R: I c cable is below I c pot.

19
19 ITER TF Conductors Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 Statistics T cs 6.5 K 3 CIC conductors 6 K T cs 6.5 K 4 CIC conductors 5.5 K T cs 6 K 5 CIC conductors T cs 5.5 K 4 CIC conductors

20
20 Summary Rainer Wesche, WAMSDO Workshop, CERN, May 19-23, 2008 For NbTi sub- and full-size conductors, a good agreement of measured T cs (I c ) with the potential values has been found. No evidence for cyclic load degradation in the two tested sub-size conductors. Nb 3 Sn sub-size: Dipole pre-prototype and PITSAM 1 show excellent agreement with potential T cs and I c. Data can be described without a load-dependent extra strain. These two conductors are not sensitive to cyclic loading. VAC triplet, PITSAM 2, PITSAM 5 short showed reduced performance after cyclic loading and/or thermal cycles. T cs and I c are below the potential values. Nb 3 Sn full-size: For TFAS1-EAS & OST, TFAS2-OCSI & OKSC, TFPRO2-OST1, JATF3 Furukawa & JASTEC and KOTF, the measured T cs values (I c ) are below the potential values. Most of these conductors are sensitive to cyclic loading. Potential values have been reached in TFPRO1-EAS1 & 2, TFPRO2-OST2. JATF1 & 2 (Hitachi and Mitsubishi) are close to the potential values. ITER conductors: 7 out of 16 reach T cs values of 6 K or above, 5 conductors are in the vicinity of the 5.7 K criterion. There remain doubts if the potential of the strands is fully used in all conductors.

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google